- Weather testing of polymers
Weather testing of polymers is the controlled
polymer degradationand polymer coatingdegradation under lab or natural conditions.
Just like errosion of rocks, natural phenomena can cause degratation in polymer systems. The elements of most concern to polymers are Ultraviolet radiation, moisture and humidity, high temperatures and temperature fluctuations. Polymers are used in every day life, so it is important for scientists and polymer produces to understand durability and expected lifespan of polymer products.
Paint, a common polymer coating, is used to change the colour, change the reflectance ( gloss), as well as forming a protective coating. The structure of paint consists of pigmentsin a matrix of resin.A typical example is painted steelroofing and walling products, which are constantly exposed to harmful weathering conditions.
Typical result of polymer surface after weathering
Figure 1.1 shows typical weathering results of a sample of painted steel; the paint on the steel is an example of a common polymer system. The sample on the left had been placed in an outdoor exposure rack, and weathered for a total of 6 years. It can be seen that the sample has a chalky appearance and has undergone a colour change in comparison to the unweathered sample on the right.
Colour is determined by light-reflecting chemical particles, pigments, in the paint. These particles can have very different physical sizes, as shown in the diagram in figure 1.2. In this example, the black pigments are the small black dots; red pigments are larger spheres, while the yellow pigments are
acicular. This combination of pigments produces the original brown colour. The upper diagram has had no weathering, and the surface is still smooth and undamaged. The lower diagram shows the painted surface after weathering has occurred. The surface has eroded with significant loss of the black and red pigments from the surface layer. The pitted surface scatters light, therefore reducing the gloss and creating the chalky affect. The larger acicular yellow pigments are more difficult to remove, resulting in a colour change towards a more yellowy appearance. Weather testing was paramount is discovering this mechanism. Pigment composition has recently been modified to help minimise this effect.
Types of weather testing
There are 3 main testing techniques; Natural Weathering, Accelerated Natural Weathering and Artificial Weathering. Because natural weathering can be a slow process, each of the techniques is a tradeoff between realistic weathering results and the duration of testing before results are collated.
Natural Weathering involves placing samples on inclined racks orientated at the
sun. In Northern hemispherethese racks are at an angle of 45 degrees in a southerly direction. In Southern hemispherethese racks are at an angle of 45 degrees in a northerly direction.This angle ensures exposure to the full spectrumof solar radiation, from infraredto Ultra violet.Sites used for this type of testing are usually in tropical areas as high temperature, UV intensity and humidity are needed for maximum degradation. Florida, for example is the world standard as it possesses all three characteristics.Despite the harsh conditions, testing takes several years before significant results are achieved.
Accelerated Natural Weathering
To speed up the weathering process while still using natural weather conditions, accelerated natural testing can be applied. One method uses mirrors to amplify available UV radiation. A device known as a Fresnel-reflecting concentrator uses photo-receptor cells to maintain alignment with the sun and 10 mirrors to reflect sunlight onto the test specimens.
Such devices, which are known by trade names Q-Trac and Emma, are typically used in Arizona and other desert locations with a high percentage of sunlight and low relative humidity. The
Arizona deserttypically provides 180 kilo Langleyper year.These exposures can be used with water spray to simulate a more humid climate. In addition, water containing up to 5% sodium chloride can be sprayed to create the conditions for corrosion to occur.
It is typical for this to accelerate weathering by a factor 5, in comparison to weathering in Florida.
An Atrac in Townsville Australia, uses follow the sun technology in which the samples are rotated so that they always face the sun. In 17 months this produced the equivalent of 2 years of weathering.
The weather testing process can be greatly accelerated through the use of specially designed weathering chambers. While this speeds up the time needed to get results, the conditions are not always representative of real world conditions. "Most of the commercialized devices are using
Gas-discharge lampor Electric arc(carbon) to simulate/accelerate the effect of sunlight. Besides fluorescent lamps where the short UV are converted into visible light with fluorescent coatings, xenon, mercury, metal halide or carbon arc lamps have to be used with a careful elimination of shorter wawelenghs usually by adding a borosilicate filter."
QUV Accelerated Weathering testing is a laboratory simulation of the damaging forces of weather for the purposes of predicting the relative durability of materials exposed to outdoor environments. Racks of samples are placed in the QUV chamber. Rain and dew systems are simulated by pressurized spray and condensation systems while damaging effects of sunlight are simulated by fluorescent UV lamps. The exposure temperature is automatically controlled. Cyclical weather conditions can also be simulated. Three types of
fluorescent lamps are commonly used for QUV. Two of these are of the type UVB (medium wavelength UV), while the third is UVA (longer wavelength UV similar to black light). All these lamps produce mostly UV as opposed to visible or infrared light. The lamp used, and therefore the wavelength of UV light produced will affect how realistic the final degradation results will be. In reality, natural sunlight contains radiation from many areas of the spectrum. This includes both UVA and UVB, however the UVB radiation is at the lowest end of natural light and is less predominant than UVA. Since it has a shorter wavelength, it also has a higher energy. This makes UVB more damaging not only because it increase chemical reaction kinetics, but also because it can initiate chemical reactions to occur which would not normally be possible under natural condition. For this reason, testing using only UVB lamps have been shown to have poor correlation relative to natural weather testing of the same samples.
"The SEPAP 12-24 has been designed, in the late seventies, by the scientists of University Blaise Pascal [http://www.univ-bpclermont.fr/LABOS/lpmm] , [http://www.cnep-ubp.com] specialists of molecular photochemistry, to provoke in accelerated controlled conditions the same chemical evolutions as those occurring at long term under the permanent physicochemical stresses of the environment, i.e. UV - heat – atmospheric oxygen and water as an aggravating agent.
"That ageing chamber based on fundamental concepts differs widely from the ageing units based on the simulation of environmental stresses in non-accelerated conditions like in some xenon based instruments.In SEPAP 12-24 :
*"the samples are rotating to insure an homogenous exposure ;"
*"the incident light is supplied by four medium-pressure
Mercury-vapor lampsfiltered by the borosilicate envelops of the lamps ; the incident light is not containing any radiations whose wavelength would be shorter than 300 nm. Although the spectral distribution is not simulating the solar light, the vibrational relaxations which occur from each excited states insure the absence of any wavelength effect under the mercury arc excitation, the light spectral distribution influencing only the rate of the photoreactions. That concept has been largely checked in the last 30 years ;"
*"since the photochemical activation (due to UV) and the thermal excitation cannot be deconjugated, it is essential to control the temperature of the samples surfaces directly exposed to light. A patented device insures that requirement in SEPAP 12-24 ;"
*"the water present in the polymeric blend exposed in SEPAP 12-24 is formed through the decomposition of the primary hydroperoxides ; no external water is brought on the exposed sample. The water effect on artificial ageing is handled either in SEPAP 12-24 H (when conjugated with the effects of UV, heat and oxygen), or through post-photochemical immersions in neutral water (in absence of conjugated effects"")" ."The durability control of polymeric formulations through the SEPAP 12-24 testing is currently required by some French and European standards and by many industrial companies (see list on [http://www.cnep-ubp.com] )"
* "ASTM STANDARDS B117": Standard Method of Salt Spray (fog) Testing,
* "ASTM D1014 (45° North)": Test method for Conducting Exterior Exposure Tests of Paints on Steel
* "ASTM G90": Standard Practice for Performing Accelerated Outdoor Weathering of Nonmetallic Materials Using Concentrated Natural Sunlight
* "ASTM G154": Standard Practice for Operating Fluorescent Light Apparatus for UV Exposure of Non-metallic Materials
* Q.U.V Accelerated Weathering Tester operation manual, Q-Lab Corporation, Cleveland, OH, USA, www.q-lab.com.
* UV Weathering and Related Test Methods, Cabot corporation, www.cabot-corp.com
*"G.C. Eastwood, A. Ledwith, S. Russo, P. Sigwalt, vol 6 ; "Polymer Reactions, vol 6" in "Comprehensive Polymer Science, Pergamon press, 1989, ISBN [0-08-036210-9] "
*"Olivier Haillant, "Polymer weathering: a mix of empiricism and science", "Material Testing Product and Technology News", 2006, 36 (76), 3-12 [http://www.atlas-mts.com] "
*"Jacques Lemaire,"Predicting polymer durability" in "Chemtech", october 1996, 42- 47."
Wikimedia Foundation. 2010.
Look at other dictionaries:
Stabilizers for polymers — are used directly or by combinations to prevent the various effects such as oxidation, chain scission and uncontrolled recombinations and cross linking reactions that are caused by photo oxidation of polymers. Polymers are considered to get… … Wikipedia
Thermal degradation of polymers — is molecular deterioration as a result of overheating. At high temperatures the components of the long chain backbone of the polymer can begin to separate (molecular scission) and react with one another to change the properties of the polymer.… … Wikipedia
Chemically Assisted Degradation of Polymers — is a type of polymer degradation that involves a change of the polymer properties due to a chemical reaction with the polymer’s surroundings. There are many different types of possible chemical reactions causing degradation however most of these… … Wikipedia
Chemically assisted degradation of polymers — is a type of polymer degradation that involves a change of the polymer properties due to a chemical reaction with the polymer’s surroundings. There are many different types of possible chemical reactions causing degradation however most of these… … Wikipedia
materials testing — Introduction measurement of the characteristics and behaviour of such substances as metals, ceramics, or plastics under various conditions. The data thus obtained can be used in specifying the suitability of materials for various… … Universalium
Photovieillissement accéléré en SEPAP — SEPAP UN OUTIL POUR ÉVALUER LA DURÉE DE VIE DES MATIÈRES PLASTIQUES * 4 lampes à vapeur de mercure de 400Watts émettant intensément entre 290 et 450nm * Un contrôle de température de la surface de l échantillon entre 45 °C et 80 … Wikipédia en Français
Ultraviolet — UV redirects here. For other uses, see UV (disambiguation). UVB redirects here. For the mysterious shortwave radio station in Russia, see UVB 76. For other uses, see Ultraviolet (disambiguation). False color image of the Sun s corona as seen in… … Wikipedia
National Centre for the Evaluation of Photoprotection — CNEP is a research center for durability prediction and failures analysis of plastics (polymer) materials. The increasing use of plastics in daily life and for high tech applications points out the necessity to improve their reliability. These… … Wikipedia
Weathering — This article is about weathering of rocks and minerals. For weathering of polymers, see Polymer degradation and Weather testing of polymers. Weathering is the breaking down of rocks, soils and minerals as well as artificial materials through… … Wikipedia
Polymer degradation — is a change in the properties tensile strength, colour, shape, etc of a polymer or polymer based product under the influence of one or more environmental factors such as heat, light or chemicals. These changes are usually undesirable, such as… … Wikipedia